LMucko/crystallography-open-database huggingface dataset:
Structures, Phase Transitions, Hydration, and Ionic Conductivity of Ba4Nb2O9
Ling, Chris D.; Avdeev, Maxim; Kutteh, Ramzi; Kharton, Vladislav V.; Yaremchenko, Aleksey A.; Fialkova, Svitlana; Sharma, Neeraj; Macquart, René B; Hoelzel, Markus; Gutmann, Matthias; Chemistry of Materials 21 (2009) 3853–; doi:10.1021/cm901644e

data_4001052
_publ_section_title
;
 Structures, Phase Transitions, Hydration, and Ionic Conductivity of
 Ba4Nb2O9
;
_journal_issue                   16
_journal_name_full               'Chemistry of Materials'
_journal_page_first              3853
_journal_paper_doi               10.1021/cm901644e
_journal_volume                  21
_journal_year                    2009
_chemical_formula_sum            'Ba6 Nb3 O13.5'
_chemical_formula_weight         1318.68
_chemical_name_systematic        ' ?'
_space_group_IT_number           190
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6c -2c'
_symmetry_space_group_name_H-M   'P -6 2 c'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            2
_cell_length_a                   10.3829(6)
_cell_length_b                   10.3829
_cell_length_c                   8.5722(8)
_cell_volume                     800.31(9)
_pd_block_id
2009-05-17T20:58|A-BA4NB2O9_1273K_phase1|Chris_Ling||
_pd_phase_name                   'alpha-Ba4Nb2O9 1273 K'
_cod_data_source_file            cm901644e_si_001.cif
_cod_data_source_block           A-BA4NB2O9_1273K_phase_1
_cod_depositor_comments
;
The following automatic conversions were performed:

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.2 from 2011-04-26 (102
times).

'_geom_angle_publ_flag' value 'N' changed to 'n' according
to /home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary
named 'cif_core.dic' version 2.4.2 from 2011-04-26 (740 times).

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_cell_volume        800.32(13)
_cod_original_formula_sum        'Ba6 Nb3.00 O13.50'
_cod_database_code               4001052
Structures, Phase Transitions, Hydration, and Ionic Conductivity of Ba4Nb2O9
Ling, Chris D.; Avdeev, Maxim; Kutteh, Ramzi; Kharton, Vladislav V.; Yaremchenko, Aleksey A.; Fialkova, Svitlana; Sharma, Neeraj; Macquart, René B; Hoelzel, Markus; Gutmann, Matthias; Chemistry of Materials 21 (2009) 3853–; doi:10.1021/cm901644e

data_4001053
_publ_section_title
;
 Structures, Phase Transitions, Hydration, and Ionic Conductivity of
 Ba4Nb2O9
;
_journal_issue                   16
_journal_name_full               'Chemistry of Materials'
_journal_page_first              3853
_journal_paper_doi               10.1021/cm901644e
_journal_volume                  21
_journal_year                    2009
_chemical_formula_sum            Nb
_chemical_formula_weight         92.91
_chemical_name_systematic        ' ?'
_space_group_IT_number           229
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            2
_cell_length_a                   3.33572(23)
_cell_length_b                   3.33572
_cell_length_c                   3.33572
_cell_volume                     37.117(3)
_pd_block_id
2009-05-17T20:58|A-BA4NB2O9_1273K_phase2|Chris_Ling||
_pd_phase_name                   Niobium
_cod_data_source_file            cm901644e_si_001.cif
_cod_data_source_block           A-BA4NB2O9_1273K_phase_2
_cod_depositor_comments
;
The following automatic conversions were performed:

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.2 from 2011-04-26 (14
times).

'_geom_angle_publ_flag' value 'N' changed to 'n' according
to /home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary
named 'cif_core.dic' version 2.4.2 from 2011-04-26 (28 times).

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_cell_volume        37.117(8)
_cod_original_sg_symbol_H-M      'I m 3 m'
_cod_database_code               4001053
Crystal Structure of Sr0.4Ce0.4TiO3Ceramics
Ubic, Rick; Subodh, Ganesanpotti; Gout, Delphine; Sebastian, Mailadil T.; Proffen, Thomas; Chemistry of Materials 21 (2009) 4706–; doi:10.1021/cm9018698

data_4001057
_publ_section_title
;
 Crystal Structure of Sr0.4Ce0.4TiO3Ceramics
;
_journal_issue                   19
_journal_name_full               'Chemistry of Materials'
_journal_page_first              4706
_journal_paper_doi               10.1021/cm9018698
_journal_volume                  21
_journal_year                    2009
_chemical_formula_sum            'Ce0.4 O3 Sr0.4 Ti'
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 125.2219
_cell_angle_gamma                90
_cell_formula_units_Z            3
_cell_length_a                   9.5228
_cell_length_b                   5.4869
_cell_length_c                   5.4818
_cell_volume                     233.990
_cod_data_source_file            cm9018698_si_001.cif
_cod_data_source_block           (I)
_cod_original_cell_volume        233.993
_cod_original_formula_sum        'Ce0.4 O3 Sr0.4 Ti1'
_cod_database_code               4001057
Unique LaTaO4Polymorph for Multiple Energy Applications
Nyman, May; Rodriguez, Mark A.; Rohwer, Lauren E.S.; Martin, James E.; Waller, Mollie; Osterloh, Frank E.; Chemistry of Materials 21 (2009) 4731–; doi:10.1021/cm9020645

data_4001063
_publ_section_title
;
 Unique LaTaO4Polymorph for Multiple Energy Applications
;
_journal_issue                   19
_journal_name_full               'Chemistry of Materials'
_journal_page_first              4731
_journal_paper_doi               10.1021/cm9020645
_journal_volume                  21
_journal_year                    2009
_chemical_formula_sum            'La O4 Ta'
_chemical_formula_weight         383.85
_chemical_name_systematic        ' ?'
_space_group_IT_number           61
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            8
_cell_length_a                   7.82857(8)
_cell_length_b                   11.21789(12)
_cell_length_c                   7.46427(8)
_cell_volume                     655.512(12)
_pd_block_id                     2009-08-07T12:16|11BMB_0615_phase1|||
_pd_phase_name                   intermedaite
_cod_data_source_file            cm9020645_si_001.cif
_cod_data_source_block           11BMB_0615_phase_1
_cod_depositor_comments
;
The following automatic conversions were performed:

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.2 from 2011-04-26 (40
times).

'_geom_angle_publ_flag' value 'N' changed to 'n' according
to /home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary
named 'cif_core.dic' version 2.4.2 from 2011-04-26 (43 times).

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_cell_volume        655.512(8)
_cod_database_code               4001063
Anion-Binding Properties of a Cyclic Pseudohexapeptide Containing 1,5-Disubstituted 1,2,3-Triazole Subunits
Martin R. Krause; Richard Goddard; Stefan Kubik; Journal of Organic Chemistry 76 (2011) 7084–7095; doi:10.1021/jo201024r

data_4026557
_publ_section_title
;
 Anion-Binding Properties of a Cyclic Pseudohexapeptide Containing
 1,5-Disubstituted 1,2,3-Triazole Subunits
;
_journal_name_full               'Journal of Organic Chemistry'
_journal_page_first              7084
_journal_page_last               7095
_journal_paper_doi               10.1021/jo201024r
_journal_volume                  76
_journal_year                    2011
_chemical_formula_sum            'C33 H39 N9 O9'
_space_group_IT_number           146
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  'R 3'
_symmetry_space_group_name_H-M   'R 3 :H'
_audit_block_code                'Spiegelbild von 3630'
_audit_creation_date             2011-05-16
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            3
_cell_length_a                   14.2352(9)
_cell_length_b                   14.2352(9)
_cell_length_c                   15.1711(9)
_cell_volume                     2662.4(3)
_cod_data_source_file            jo201024r_si_004_2.cif
_cod_data_source_block           inv3630
_cod_original_sg_symbol_H-M      'R 3'
_cod_database_code               4026557
Iron displacements and magnetoelastic coupling in the antiferromagnetic spin-ladder compound BaFe_{2}Se_{3}
Caron, J.; Neilson, J.; Miller, D.; Llobet, A.; McQueen, T.; Physical Review B 84 (2011) 180409–; doi:10.1103/PhysRevB.84.180409

data_1504313
_publ_contact_author_address
'Dept. of Chemistry, Johns Hopkins University'
_publ_contact_author_email       mcqueen@jhu.edu
_publ_contact_author_name        'Tyrel M. McQueen'
_publ_section_title
;
 Iron displacements and magnetoelastic coupling in the antiferromagnetic
 spin-ladder compound BaFe_{2}Se_{3}
;
_journal_issue                   18
_journal_name_full               'Physical Review B'
_journal_page_first              180409
_journal_paper_doi               10.1103/PhysRevB.84.180409
_journal_volume                  84
_journal_year                    2011
_chemical_formula_sum            'Ba Fe2 Se3'
_chemical_formula_weight         485.90
_chemical_name_common            'Barium Iron Selenide'
_chemical_name_systematic        'Barium Diiron(II) Triselenide'
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            4
_cell_length_a                   11.9996(23)
_cell_length_b                   5.4711(10)
_cell_length_c                   9.2156(18)
_cell_volume                     605.0(2)
_computing_structure_refinement  GSAS
_diffrn_ambient_temperature      300
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     white-beam
_diffrn_radiation_wavelength_details
'Time-of-Flight Neutron, HIPD, Lujan-LANSCE-Los Alamos'
_exptl_crystal_density_diffrn    5.335
_refine_ls_goodness_of_fit_all   1.96
_refine_ls_matrix_type           full
_refine_ls_number_parameters     89
_refine_ls_number_restraints     0
_refine_ls_shift/su_max          0.07
_refine_ls_shift/su_mean         0.01
_cod_data_source_file            BaFe2Se3_300K_ICSD.cif
_cod_data_source_block           BaFe2Se3_300K_publ
_cod_original_cell_volume        605.02(34)
_cod_database_code               1504313
Iron displacements and magnetoelastic coupling in the antiferromagnetic spin-ladder compound BaFe_{2}Se_{3}
Caron, J.; Neilson, J.; Miller, D.; Llobet, A.; McQueen, T.; Physical Review B 84 (2011) 180409–; doi:10.1103/PhysRevB.84.180409

data_1504314
_publ_contact_author_address
'Dept. of Chemistry, Johns Hopkins University'
_publ_contact_author_email       mcqueen@jhu.edu
_publ_contact_author_name        'Tyrel M. McQueen'
_publ_section_title
;
 Iron displacements and magnetoelastic coupling in the antiferromagnetic
 spin-ladder compound BaFe_{2}Se_{3}
;
_journal_issue                   18
_journal_name_full               'Physical Review B'
_journal_page_first              180409
_journal_paper_doi               10.1103/PhysRevB.84.180409
_journal_volume                  84
_journal_year                    2011
_chemical_formula_sum            'Ba Fe2 Se3'
_chemical_formula_weight         485.90
_chemical_name_common            'Barium Iron Selenide'
_chemical_name_systematic        'Barium Diiron(II) Triselenide'
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90.00000
_cell_angle_beta                 90.00000
_cell_angle_gamma                90.00000
_cell_formula_units_Z            4
_cell_length_a                   11.88345(24)
_cell_length_b                   5.41411(10)
_cell_length_c                   9.14086(20)
_cell_volume                     588.11(2)
_computing_structure_refinement  FULLPROF
_diffrn_ambient_temperature      5
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     white-beam
_diffrn_radiation_wavelength_details
'Time-of-Flight Neutron, HIPD, Lujan-LANSCE-Los Alamos'
_exptl_crystal_density_diffrn    5.488
_refine_ls_goodness_of_fit_all   0.132
_refine_ls_matrix_type           full
_refine_ls_number_parameters     68
_refine_ls_number_restraints     0
_refine_ls_shift/su_max          0.1
_refine_ls_shift/su_mean         0.03
_cod_data_source_file            BaFe2Se3_5K_ICSD.cif
_cod_data_source_block           BaFe2Se3_5K_publ
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Orthorhombic' changed to
'orthorhombic' according to the built-in table from CIF Core
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_cell_volume        588.10797
_cod_database_code               1504314
Molecular Growth of Polyoxometalate Architectures Based on [−Ag{Mo8}Ag−] Synthons: Toward Designed Cluster Assemblies
Abbas, Hamera; Streb, Carsten; Pickering, Alexandra L.; Neil, Andrew R.; Long, De-Liang; Cronin, Leroy; Crystal Growth & Design 8 (2008) 635–; doi:10.1021/cg700736v

data_4503202
_publ_section_title
;
 Molecular Growth of Polyoxometalate Architectures Based on
 [&#x2212;Ag{Mo8}Ag&#x2212;] Synthons: Toward Designed Cluster Assemblies
;
_journal_issue                   2
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              635
_journal_paper_doi               10.1021/cg700736v
_journal_volume                  8
_journal_year                    2008
_chemical_formula_sum            'C18 Ag4 Mo8 N6 O32'
_chemical_formula_weight         2011.212
_chemical_name_common
;
Compound AN16
;
_space_group_IT_number           2
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_audit_creation_date             07-04-13
_audit_creation_method
'Created with Diamond (www.crystalimpact.com)'
_audit_update_record             07-04-13
_cell_angle_alpha                63.312(1)
_cell_angle_beta                 76.600(2)
_cell_angle_gamma                88.951(1)
_cell_formula_units_Z            1
_cell_length_a                   10.1101(2)
_cell_length_b                   11.4232(3)
_cell_length_c                   11.5474(3)
_cell_volume                     1153.43(5)
_refine_ls_R_factor_all          0.025
_cod_data_source_file            cg700736v-file005.cif
_cod_data_source_block           AN16
_cod_original_cell_volume        1153.4(1)
_cod_original_sg_symbol_Hall     -P_1
_cod_original_formula_sum        'Ag4 Mo8 O32 N6 C18'
_cod_database_code               4503202
Molecular Growth of Polyoxometalate Architectures Based on [−Ag{Mo8}Ag−] Synthons: Toward Designed Cluster Assemblies
Abbas, Hamera; Streb, Carsten; Pickering, Alexandra L.; Neil, Andrew R.; Long, De-Liang; Cronin, Leroy; Crystal Growth & Design 8 (2008) 635–; doi:10.1021/cg700736v

data_4503203
_publ_section_title
;
 Molecular Growth of Polyoxometalate Architectures Based on
 [&#x2212;Ag{Mo8}Ag&#x2212;] Synthons: Toward Designed Cluster Assemblies
;
_journal_issue                   2
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              635
_journal_paper_doi               10.1021/cg700736v
_journal_volume                  8
_journal_year                    2008
_chemical_formula_sum            'Ag4 Mo8 O32'
_chemical_formula_weight         1710.974
_chemical_name_common
;
Compound AN16
;
_space_group_IT_number           2
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_audit_creation_date             07-04-13
_audit_creation_method
'Created with Diamond (www.crystalimpact.com)'
_audit_update_record             07-04-13
_cell_angle_alpha                63.312(1)
_cell_angle_beta                 76.600(2)
_cell_angle_gamma                88.951(1)
_cell_formula_units_Z            1
_cell_length_a                   10.1101(2)
_cell_length_b                   11.4232(3)
_cell_length_c                   11.5474(3)
_cell_volume                     1153.43(5)
_refine_ls_R_factor_all          0.025
_cod_data_source_file            cg700736v-file005.cif
_cod_data_source_block           AN16
_cod_original_cell_volume        1153.4(1)
_cod_original_sg_symbol_Hall     -P_1
_cod_database_code               4503203
Phase Transitions and CO2Adsorption Properties of Polymeric Magnesium Formate
Rossin, Andrea; Ienco, Andrea; Costantino, Ferdinando; Montini, Tiziano; Di Credico, Barbara; Caporali, Maria; Gonsalvi, Luca; Fornasiero, Paolo; Peruzzini, Maurizio; Crystal Growth & Design 8 (2008) 3302–; doi:10.1021/cg800181q

data_4503635
_publ_section_title
;
 Phase Transitions and CO2Adsorption Properties of Polymeric Magnesium
 Formate
;
_journal_issue                   9
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              3302
_journal_paper_doi               10.1021/cg800181q
_journal_volume                  8
_journal_year                    2008
_chemical_formula_sum            'C2 Mg O6'
_chemical_formula_weight         144.32
_chemical_name_systematic        ' ?'
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90.0
_cell_angle_beta                 98.1659(30)
_cell_angle_gamma                90.0
_cell_formula_units_Z            4
_cell_length_a                   8.65107(31)
_cell_length_b                   7.15222(25)
_cell_length_c                   9.4041(4)
_cell_volume                     575.97(4)
_pd_block_id
2009-02-27T12:48|2H2O_2_phase1|erdinando_costantino||
_pd_phase_name
'from C:/Documents and Settings/FERDINANDO/Documenti/ferdinando/lav'
_cod_data_source_file            cg800181q-file005.cif
_cod_data_source_block           2H2O_2_phase_1
_cod_depositor_comments
;
The following automatic conversions were performed:

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (33
times).

'_geom_angle_publ_flag' value 'N' changed to 'n' according
to /home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary
named 'cif_core.dic' version 2.4.1 from 2010-06-29 (36 times).

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_database_code               4503635
Novel Trigonal ZrWMoO8Structure and Its Transformations
Deng, Xuebin; Tao, Juzhou; Yang, Xiaojing; Ma, Hui; Richardson, James W.; Zhao, Xinhua; Chemistry of Materials 20 (2008) 1733–; doi:10.1021/cm071605y

data_4001085
_publ_section_title
;
 Novel Trigonal ZrWMoO8Structure and Its Transformations
;
_journal_issue                   5
_journal_name_full               'Chemistry of Materials'
_journal_page_first              1733
_journal_paper_doi               10.1021/cm071605y
_journal_volume                  20
_journal_year                    2008
_chemical_formula_sum            'Mo O8 W Zr'
_chemical_formula_weight         499.00
_space_group_IT_number           164
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-P 3 2"'
_symmetry_space_group_name_H-M   'P -3 m 1'
_audit_creation_date             2006-06-29T21:52
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
' 2006-06-29T21:52  Initial CIF as created by GSAS2CIF'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            1
_cell_length_a                   5.84039(10)
_cell_length_b                   5.84039
_cell_length_c                   6.06707(17)
_cell_volume                     179.223(6)
_computing_structure_refinement  GSAS
_diffrn_radiation_polarisn_ratio 0.5
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Cu K\a'
_diffrn_radiation_wavelength     1.541874
_pd_block_id                     2006-06-29T21:52|TRI750|tri750|tri750
_pd_phase_name                   tri750
_pd_proc_ls_prof_R_factor        0.0588
_pd_proc_ls_prof_wR_expected     0.0280
_pd_proc_ls_prof_wR_factor       0.0830
_refine_ls_goodness_of_fit_all   2.98
_refine_ls_matrix_type           full
_refine_ls_number_parameters     34
_refine_ls_number_restraints     0
_refine_ls_R_Fsqd_factor         0.08807
_refine_ls_shift/su_max          0.05
_refine_ls_shift/su_mean         0.00
_cod_data_source_file            cm071605y-file001.cif
_cod_data_source_block           TRI750_publ
_cod_depositor_comments
;
The following automatic conversions were performed:

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (19
times).

'_geom_angle_publ_flag' value 'N' changed to 'n' according
to /home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary
named 'cif_core.dic' version 2.4.1 from 2010-06-29 (31 time).

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_cell_volume        179.223(7)
_cod_original_sg_symbol_H-M      'p -3 m 1'
_cod_original_formula_sum        'Mo1.00 O8 W1.00 Zr'
_cod_database_code               4001085